Download ASTM A228-A228M-14 Standard Specification for Steel Wire, Music Spring Quality.pdf...
Designation: A228/A228M − 14
Standard Specification for
Steel Wire, Music Spring Quality1 This standard is issued under the fixed designation A228/A228M; the number immediately following the designation indicates the year of original adoption or, in the case of revision, the year of last revision. A number in parentheses indicates the year of last reapproval. A superscript epsilon (´) indicates an editorial change since the last revision or reapproval. This standard has been approved for use by agencies of the U.S. Department of Defense.
2.2 Federal Standard: Fed. Std. No. 123, Marking for Shipment (Civil Agencies)4 2.3 American National Standard:5 B32.4 Preferred Metric Sizes for Round, Square, Rectangle, and Hexagon Metal Products 2.4 AIAG Standard:6 AIAG B-5 02.00 Primary Metals Identification Tag Application Standard
1.1 This specification covers a high quality, round, colddrawn steel music spring quality wire, uniform in mechanical properties, intended especially for the manufacture of springs subject to high stresses or requiring good fatigue properties. 1.2 The values stated in either SI units or inch-pound units are to be regarded separately as standard. The values stated in each system may not be exact equivalents; therefore, each system shall be used independently of the other. Combining values from the two systems may result in non-conformance with the standard.
3. Terminology 3.1 Definitions—For definitions of terms used in this specification, refer to Terminology A941.
2. Referenced Documents
4. Ordering Information
2.1 ASTM Standards:2 A370 Test Methods and Definitions for Mechanical Testing of Steel Products A510/A510M Specification for General Requirements for Wire Rods and Coarse Round Wire, Carbon Steel A700 Practices for Packaging, Marking, and Loading Methods for Steel Products for Shipment (Withdrawn 2014)3 A751 Test Methods, Practices, and Terminology for Chemical Analysis of Steel Products A938 Test Method for Torsion Testing of Wire A941 Terminology Relating to Steel, Stainless Steel, Related Alloys, and Ferroalloys E29 Practice for Using Significant Digits in Test Data to Determine Conformance with Specifications E1077 Test Methods for Estimating the Depth of Decarburization of Steel Specimens
4.1 Orders for steel wire under this specification shall contain the following information: 4.1.1 Quantity (weight in lbs, or mass in kg), 4.1.2 Name of material (music steel spring wire), 4.1.3 Diameter (Table 1 and Section 9), 4.1.4 Finish (see 10.2), 4.1.5 Packaging (Section 15), and 4.1.6 ASTM designation and year of issue. 4.2 The purchaser shall have the option to specify additional requirements, including but not limited to: 4.2.1 Requirements for certifications, heat, or test reports, (see Section 14), 4.2.2 Special packing, marking, and loading requirements (see Section 15), and 4.2.3 Other special requirements, if any, NOTE 1—A typical inch-pound units ordering description is as follows: 10 000 lb Music Steel Spring Wire, 0.055 in. diameter, phosphate coated in 1000 lb coils to ASTM A288M_A228M dated _____, or for metric units, 5000 kg Music Steel Spring Wire, 1.40 mm diameter, phosphate coated in 500 kg coils to ASTM A288 dated _____.
1 This specification is under the jurisdiction of ASTM Committee A01 on Steel, Stainless Steel and Related Alloys and is the direct responsibility of Subcommittee A01.03 on Steel Rod and Wire. Current edition approved March 1, 2014. Published April 2014. Originally approved in 1939. Last previous edition approved in 2007 as A228/A228M – 07. DOI: 10.1520/A0228_A0228M-14. 2 For referenced ASTM standards, visit the ASTM website, www.astm.org, or contact ASTM Customer Service at [email protected]
For Annual Book of ASTM Standards volume information, refer to the standard’s Document Summary page on the ASTM website. 3 The last approved version of this historical standard is referenced on www.astm.org.
4 Available from Standardization Documents Order Desk, DODSSP, Bldg. 4, Section D, 700 Robbins Ave., Philadelphia, PA 19111–5098, http:// www.dodssp.daps.mil. 5 Available from American National Standards Institute (ANSI), 25 W. 43rd St., 4th Floor, New York, NY 10036, http://www.ansi.org. 6 Available from Automotive Industry Action Group (AIAG), 26200 Lahser Rd., Suite 200, Southfield, MI 48033, http://www.aiag.org.
Copyright © ASTM International, 100 Barr Harbor Drive, PO Box C700, West Conshohocken, PA 19428-2959. United States
A228/A228M − 14 TABLE 1 Tensile Requirements
5.2 The finished wire shall be free from detrimental pipe and undue segregation.
Inch-Pound Units Diameter, in.A
0.004 0.005 0.006 0.007 0.008 0.009 0.010 0.011 0.012 0.013 0.014 0.015 0.016 0.018 0.020 0.022 0.024 0.026 0.028 0.030 0.032 0.034 0.036 0.038 0.040 0.042 0.045 0.048 0.051 0.055
Tensile Strength, ksi min max 439 426 415 407 399 393 387 382 377 373 369 365 362 356 350 345 341 337 333 330 327 324 321 318 315 313 309 306 303 300
485 471 459 449 441 434 428 422 417 412 408 404 400 393 387 382 377 373 368 365 361 358 355 352 349 346 342 339 335 331
0.059 0.063 0.067 0.072 0.076 0.080 0.085 0.090 0.095 0.100 0.102 0.107 0.110 0.112 0.121 0.125 0.130 0.135 0.140 0.145 0.150 0.156 0.162 0.177 0.192 0.207 0.225 0.250 0.262 0.283
5.3 The wire shall be cold drawn to produce the desired mechanical properties.
Tensile Strength, ksi min max 296 293 290 287 284 282 279 276 274 271 270 268 267 266 263 261 259 258 256 254 253 251 249 245 241 238 235 230 228 223
6. Chemical Composition
327 324 321 317 314 312 308 305 303 300 299 296 295 294 290 288 286 285 283 281 279 277 275 270 267 264 260 255 253 248
6.1 The steel shall conform to the requirements for chemical composition prescribed in Table 2. 6.2 Heat Analysis—Each heat of steel shall be analyzed by the manufacturer to determine the percentage of elements prescribed in Table 2. This analysis shall be made from a test specimen preferably taken during the pouring of the heat. When requested in the purchase order, the heat analysis shall be reported to the purchaser. 6.3 Product Analysis—An analysis may be made by the purchaser from finished wire representing each heat of steel. The chemical composition thus determined, as to elements required or restricted, shall conform to the product analysis requirements specified in Table 7 of Specification A510/ A510M. 6.4 For referee purposes, Test Methods, Practices, and Terminology A751 shall be used. 7. Mechanical Properties 7.1 Tension Test: 7.1.1 Requirements—The material as represented by tension test specimens shall conform to the requirements prescribed in Table 1. 7.1.2 Number of Tests—One test specimen shall be taken from the top or outside end of each coil, reel, or spool, and shall be tested for conformance. 7.1.3 Test Method—The tension test shall be made in accordance with Test Methods and Definitions A370. 7.1.4 For wire diameters over 0.283 in. [7.2 mm], mechanical properties shall be negotiated between purchaser and supplier and shall be included on the order information.
SI Units Diameter, mmA 0.10 0.11 0.12 0.14 0.16 0.18 0.20 0.22 0.25 0.28 0.30 0.35 0.40 0.45 0.50 0.55 0.60 0.65 0.70 0.80 0.90 1.00 A
Tensile Strength, MPa min max 3000 2950 2900 2850 2800 2750 2700 2680 2650 2620 2600 2550 2500 2450 2400 2380 2350 2320 2300 2250 2200 2150
3300 3250 3200 3150 3100 3050 3000 2980 2950 2920 2900 2820 2750 2700 2650 2620 2600 2580 2550 2500 2450 2400
1.1 1.2 1.4 1.6 1.8 2.0 2.2 2.5 2.8 3.0 3.2 3.5 3.8 4.0 4.5 5.0 5.5 6.0 6.5 7.0 7.2
Tensile Strength, MPa min max 2120 2100 2050 2000 1980 1950 1900 1850 1820 1800 1780 1750 1720 1700 1680 1650 1620 1600 1580 1550 1540
2380 2350 2300 2250 2220 2200 2150 2100 2050 2000 1980 1950 1920 1900 1880 1850 1820 1800 1780 1750 1740
7.2 Wrap Test: 7.2.1 Requirements—The material shall conform to the requirements prescribed in Table 3. The requirement for conformance to wrap test on wires above 0.283 in. [7.2 mm] in diameter shall be agreed upon between purchaser and producer. 7.2.2 Number of Tests—One test specimen shall be taken from the top or outside end of each coil, reel or spool and shall be tested for conformance. 7.2.3 Test Method—Each test specimen shall be closed wound on an arbor as prescribed in Table 3 for a minimum of four full wraps. Wire so tested shall not show any splits or fractures.
Tensile strength values for intermediate diameters may be interpolated.
TABLE 2 Chemical Requirements Element
5. Materials and Manufacture
Carbon Manganese Phosphorus, max Sulfur, max Silicon
5.1 The steel may be made by any commercially accepted steel-making process. The rod to be used in the manufacture of wire furnished to this specification shall be in accordance with Specification A510/A510M. 2
Composition, % 0.70–1.00 0.20–0.70 0.025 0.030 0.10–0.30
A228/A228M − 14 TABLE 3 Wrap Test Requirements
7.3.6 For wire diameters over 0.283 in. [7.2 mm], the requirement for torsion testing shall be negotiated between purchaser and supplier and shall be included on the order information.
Inch-Pound Units Diameter, in.
Less than 0.028 0.028 to 0.256, incl Over 0.256 to 0.283, incl
1× 2× 3×
8. Metallurgical Requirements 8.1 Surface Condition: 8.1.1 The surface of the wire as-received shall be free of rust, excessive scale, die marks, pits, and scratches detrimental to the end application. Seams shall not exceed 2 % of the wire diameter or 0.15 mm [0.006 in.], whichever is less. 8.1.2 Location of Test—Test specimens shall be taken from either or both ends of the coil.
SI Units Diameter, mm
Less than 0.70 0.70 to 6.5, incl Over 6.5 to 7.2, incl
1× 2× 3×
7.3 Torsion Test: 7.3.1 Requirements—The torsion test shall be applied to wire sizes 0.70 mm [0.028 in.] and larger in diameter. For wire sizes smaller in diameter than 0.70 mm [0.028 in.], the torsion test may be substituted for the wrap test (7.2). In this case, the minimum number of torsions to failure will be equivalent to 25 in a test length of 100d. 7.3.2 Number of tests—One test specimen shall be taken from the top or outside end of each coil, reel, or spool and shall be tested for conformance. 7.3.3 Test Method—Test specimens shall be prepared and tested as shown in A938 with the following exception. The minimum number of torsions (twists) to failure in a test length of 100d (where d = the wire diameter being tested) are shown in Table 4. 7.3.4 Following completion of the torsion test, the torsion fracture shall be perpendicular to the longitudinal axis of the test specimen and the surface of the test specimen shall not be split. Secondary (recoil) fractures shall be ignored. 7.3.5 Test lengths other than 100d may be utilized. In this case, the minimum number of torsions to failure shall be adjusted in direct proportion to the change in test length as determined by the following formula: Tx 5
where Tx = Td = Lx = Ld =
Td 3 Lx Ld
8.2 Decarburization: 8.2.1 The maximum affected depth of decarburization shall not exceed 2 % of the wire diameter or 0.15 mm [0.006 in.], whichever is less. The maximum average partial decarburization depth shall not exceed 1.5% of the wire diameter when measured using the test method described in 8.2.3. 8.2.2 Test Method—Decarburization shall be determined by etching a suitably polished transverse section of wire with nital. The entire periphery to be examined should be in a single plane with no edge rounding. (See Test Method E1077.) 8.2.3 The entire periphery shall be examined at a magnification of no less than 100× for depth of free ferrite and maximum affected depth. Smaller wire sizes may require higher magnification. Complete decarburization exists when only free ferrite is present. The worst case location shall be used to position perpendicular bisectors as shown in Fig. 1. The depth of decarburization (D) shall be measured at each of the four points where the perpendicular bisectors cross the circumference of the wire. The four readings so obtained shall be averaged, and the average shall not exceed 1.5% of the wire diameter. 8.2.4 The purchaser may specify more restrictive decarburization requirements where necessary for special applications.
minimum number of torsions for new test length, minimum number of torsions for 100d test length, new test length, and 100d test length
TABLE 4 Number of Torsions to Failure for Torsion Test Inch-Pound Units Diameter, in.
Number of Torsions in 100d
0.028 to 0.079, incl over 0.079 to 0.138, incl over 0.138 to 0.283, incl
25 20 15 SI Units
Number of Torsions in 100d
0.70 to 2.0, incl over 2.0 to 3.5, incl over 3.5 to 7.2, incl
25 20 15
FIG. 1 Positioning of Perpendicular Bisectors
A228/A228M − 14 all inspection and test requirements specified in this specification. Except as otherwise specified in the contract or purchase order, the manufacturer may use his own or any other suitable facilities for the performance of the inspection and test requirements unless disapproved by the purchaser at the time the order is placed. The purchaser shall have the right to perform any of the inspections and tests set forth in this specification when such inspections and tests are deemed necessary to assure that the material conforms to prescribed requirements.
These requirements shall be negotiated between the purchaser and supplier and must be included in the order information. 8.2.5 There are no decarburization requirements for wire sizes smaller in diameter than 2.0 mm [0.078 in]. 9. Dimensions and Permissible Variations 9.1 The permissible variations in the diameter of the wire shall be as specified in Table 5. 10. Workmanship, Finish, and Appearance 10.1 Workmanship—The wire shall not be kinked or improperly cast. To test for cast, one convolution of wire shall be cut from the coil, reel, or spool and placed on a flat surface. The wire shall not spring up nor show a wavy condition. Wire below 4.0 mm or 0.156 in. diameter shall lie flat while wire diameters larger than the above shall lie substantially flat. 10.1.1 Each coil, reel, or spool shall be one continuous length of wire, properly coiled and firmly tied. 10.1.2 Welds made prior to cold drawing are permitted. If unmarked welds are unacceptable to the purchaser, special arrangements should be made with the manufacturer at the time of purchase.
13. Rejection and Rehearing 13.1 Unless otherwise specified, any rejection based on tests made in accordance with these specifications shall be reported to the manufacturer as soon as possible so that an investigation may be initiated. 13.2 The material shall be adequately protected and identified correctly for the manufacturer to make a proper investigation. 14. Certification 14.1 When specified in the purchase order or contract, a producer’s or supplier’s certification shall be furnished to the purchaser that the material was manufactured, sampled, tested, and inspected in accordance with this specification and has been found to meet the requirements. When specified in the purchase order or contract, a report of the test results shall be furnished.
10.2 Finish—Music wire is supplied with many different types of finish such as bright, phosphate, tin, and others. Finish desired should be specified on purchase orders. 11. Retests 11.1 If any test specimen exhibits obvious defects or shows the presence of a weld, it shall be discarded and another specimen substituted.
14.2 The certification shall include the specification number, year date of issue, and revision letter, if any.
12. Inspection 12.1 Unless otherwise specified in the contract or purchase order, the manufacturer is responsible for the performance of
15. Packaging, Marking, and Loading for Shipment 15.1 The coil, reel or spool mass, dimensions, and the method of packaging shall be agreed upon between the manufacturer and purchaser.
TABLE 5 Permissible Variations in Wire DiameterA SI Units
to 0.25, incl Over 0.25 to Over 0.70 to Over 1.50 to Over 2.00 to Over 6.00
0.70, 1.50, 2.00, 6.00,
incl incl incl incl
Permissible Variations, plus and minus, mm
Permissible Out-of-Round, max mm
0.005 0.008 0.010 0.013 0.03 0.04
0.005 0.008 0.010 0.013 0.03 0.04
15.2 A tag shall be attached securely to each coil of wire with identifying information as agreed upon by the purchaser and manufacturer. 15.3 Unless otherwise specified in the purchaser’s order, packaging, marking, and loading for shipments shall be in accordance with those procedures recommended by Practices A700. 15.4 For Government Procurement: 15.4.1 Marking for shipment of material for civil agencies shall be in accordance with Fed. Std No. 123.
0.004 to 0.010, incl Over 0.010 to 0.028, Over 0.028 to 0.063, Over 0.063 to 0.080, Over 0.080 to 0.250, Over 0.250
incl incl incl incl
Permissible Variations, plus and minus, in.
Permissible Out-of-Round, max in.
0.0002 0.0003 0.0004 0.0005 0.001 0.0015
0.0002 0.0003 0.0004 0.0005 0.001 0.0015
15.5 Bar Coding—In addition to the previously-stated identification requirements, bar coding is acceptable as a supplementary identification method. Bar coding should be consistent with AIAG Standard 02.00, Primary Metals Identification Tag Application. The bar code may be applied to a substantially affixed tag.
A For purposes of determining conformance with this specification, all specified limits are absolute as defined in Practice E29.
16. Keywords 16.1 music spring; wire
A228/A228M − 14 ASTM International takes no position respecting the validity of any patent rights asserted in connection with any item mentioned in this standard. Users of this standard are expressly advised that determination of the validity of any such patent rights, and the risk of infringement of such rights, are entirely their own responsibility. This standard is subject to revision at any time by the responsible technical committee and must be reviewed every five years and if not revised, either reapproved or withdrawn. Your comments are invited either for revision of this standard or for additional standards and should be addressed to ASTM International Headquarters. Your comments will receive careful consideration at a meeting of the responsible technical committee, which you may attend. If you feel that your comments have not received a fair hearing you should make your views known to the ASTM Committee on Standards, at the address shown below. This standard is copyrighted by ASTM International, 100 Barr Harbor Drive, PO Box C700, West Conshohocken, PA 19428-2959, United States. Individual reprints (single or multiple copies) of this standard may be obtained by contacting ASTM at the above address or at 610-832-9585 (phone), 610-832-9555 (fax), or [email protected]
(e-mail); or through the ASTM website (www.astm.org). Permission rights to photocopy the standard may also be secured from the Copyright Clearance Center, 222 Rosewood Drive, Danvers, MA 01923, Tel: (978) 646-2600; http://www.copyright.com/